Structural Grades of Timber by Bending and Compression Tests Jorge Branco 1,a, Humberto Varum 2,b and Paulo Cruz 1,c


 Jared Kelly
 3 months ago
 Views:
Transcription
1 Structural Grades of Timber by Bending and Compression Tests Jorge Branco 1,a, Humberto Varum 2,b and Paulo Cruz 1,c 1 DECivil Engineering School, Campus de Azurém, Guimarães, Portugal 2 DECivil, Campus Universitário de Santiago, Aveiro, Portugal a b c Keywords: Timber, structural grades, mechanical tests, bending and compression Abstract. This paper presents the results obtained in a series of tests on Pinus Pinaster Ait. timber specimens, using the pren408:2000, to estimate the local and global Young s modulus and strength both in bending and compression parallel to the grain. The results obtained are compared with the values presented in the Portuguese Nationally Determined Parameters of Eurocode 5, for the quality classes assign by Portuguese Standard NP4305:1994 by visual grading. Introduction The results achieved in any assessment of mechanical properties are function of the testing method adopted. Timber mechanical properties depend of various factors, as for instance: load duration, moisture content, span, depth of the section, etc. Therefore, to accomplish the comparison between the results obtained in different laboratories, a standardization of the test procedure is required. Moreover, with the adoption of limit state design and with the development of both visual and machine stress grading, attention will be increasingly focused on the determination and monitoring of the strength properties and variability of structural grades of timber. The pren408:2000 European Standard specifies laboratory methods for the determination of some physical and mechanical properties in structural sizes. This standard presents test methods for determining the modulus of elasticity, the bending strength and the compression strength in a parallel direction to the grain orientation in structural timber. In addition, the determination of dimensions, moisture content and density are specified. In follow the bending and compression tests procedure adopted by pren408:2000 are described. Bending Test. This test use a piece simply supported with a span of 18 times the depth with the loads points placed on the third of the span, as it is shown in Fig. 1. Small steel plates of length not greater than onehalf of the depth of the test piece may be inserted between the piece and the loading heads supports to minimize local indentation. >h/2 a = 6h 6h 6h F/2 l = 5h F/2 1 >h/2 l = 18h Fig. 1  Test arrangement of the bending test The evaluation of the modulus of elasticity in bending is based on the deformations measured at the centre of a central gauge length of 5 times the depth of the section. This deformation shall be taken as the average of measurements on both faces at the neural axis. w h
2 The local modulus of elasticity in bending (E m,l )is obtained from the follow equation: 2 al1 F E m, l =. (1) 16 I w where F is an increment of load on the straightline portion of the load deformation curve (N), w is the increment of deformation corresponding (mm), a is the distance between a loading position and the nearest support (mm), l 1 is the gauge length (mm) and I is the second moment of area (mm 4 ). Using the deformation value measured at the centre of the span and at the centre of the compression or tension edge we can also calculate the value of the global modulus of elasticity in bending. Thus, the global modulus of elasticity in bending (E m,g ) is obtained from the follow equation: 3 3 l F 3a a E m, g = 3. (2) b h w 4l l where b and h are the width and depth of the cross section (mm), respectively, l is the span (mm). The bending strength is obtained with the continuation of the test just to failure, applying the load with a constant loadinghead movement so adjust that maximum load is reached within (300±120)s. Therefore, the bending strength (f m ) is given by: a Fmax f m =. (3) 2W where F max is the maximum load (N) and W is the section modulus (mm 3 ). Compression Test. In this test, the test piece shall be of full cross section, and shall have a length of 6 times the smaller crosssectional dimension. The end surfaces shall be accurately prepared to ensure that they are plane and parallel to one another and perpendicular to the axis of the piece. The load shall be applied concentrically using spherical seated loading heads permitting the application of a compressive load without inducing bending. Deformation shall be measured over a central gauge length of 4 times the smaller crosssectional dimension of the piece, using two mechanical strain gauges positioned in such way that the eventual effects of distortion shall be minimized. The modulus of elasticity in compression parallel to the grain (E c,0 ) is given as the result of: l F E c = 1, 0. (4) A w where A is the crosssectional area (mm 2 ). The compression strength is obtained with the increment of the load, applied at a constant loadinghead movement so adjusted that maximum load (F max ) is reached within (300±120)s. The compression strength (f c,0 ) is taken as the result of the follow equation: Fmax f c, 0 =. (5) A The mode of fracture and growth characteristics at the fracture section of each test piece shall be reported. Experimental Activity The experimental program is based on Pinus pinaster Ait. specimens classified as belonging to quality class EE in result of a visual strength grading conducted following the National Standard NP 4305:1995 [2]. In both tests kinds conducted, the failure time was register and the moisture content of each specimen was measure with an electronic thermohygrometer for wood. The tests
3 were carried out at the Structural Laboratory of the Civil Engineering Department of the Minho University. Bending Tests. Four beams with a cross section of 80x105 mm 2 and 1.95 m length were evaluated by fourpoints bending tests using a test arrangement following pren 408:2000 (see Fig. 1). A displacement control procedure (0.14 mm/s) with an actuator having a capacity of 100 kn has been used. In each test, apart the registration of the deformations measured at the centre of a central gauge length of 5 times the depth of the section, the deformations at the centre of the span at the centre of the tension side edge were measured. With the deformations values corresponding to the elastic deformation the calculation of the local and global values of the modulus of elasticity in bending were possible. Incrementing the load, it was also possible to obtain the bending strength as it was previously explained (Eq. 3). The bending tests results founded are presented in Table 1. Table 1 Bending tests results Beam Moisture (%) F max (kn) Time (s) E m,l (N/mm 2 ) E m,g (N/mm 2 ) f m (N/mm 2 ) B B B B Mean CoV Like it was expected, the local value for the modulus of elasticity (E m,l ) was always higher than the global value (E m,g ) as no shear deformation is taken into account in first value contrarily to the second. However the pleasants coefficients of variance (CoV) presented by both modulus of elasticity (E m,l = 0.16 and E m,g = 0.11), beam B4 did not reached the bending strength level presented by the others beams. As Fig. 2 show, the maximum load reached by B4 stay quite far from the others results, with direct consequences in the bending strength CoV (0.27). 20 Load (kn) Midspan deformation (mm) Fig. 2 Midspan deformation vs load curves obtained in the bending tests B1 B2 B3 B4 Compression Tests. Four specimens of 80x105x480 mm 3 were used in the compression tests conducted in accordance with the recommendations presented by pren 408:2000. The tests were performed under displacement control with a velocity of 0.01 mm/s using a load cell of 500 kn. Two mechanical strain gauges (one in each the two bigger crosssectional dimensions) were used to measure the deformations and one additional LVDT (Linear Variable Displacement Transducer) was placed in the loading head of the test machine, measuring thereby the grain displacement
4 presented by the specimens. After the moisture content measurement, the specimens were tested with a correct loading head movement (all the failure were reached within 300±120s). Base in the mean values of the deformation measured by the two mechanical strain gauges (in the range of elastic deformation) it was possible to calculated the modulus elasticity (E c,0 ) and with the maximum load value the calculation of the compression strength (f c,0 ). Table 2 shows the compression tests results carried out. Table 2 Compression tests results Specimen Moisture (%) Time (s) F max (kn) E c,0 (N/mm 2 ) f c,0 (N/mm 2 ) S S S S Mean CoV It is clearly show by the results achieved that the compression behaviour of timber is quite heterogeneous. The coefficient of variance presented by the modulus of elasticity and strength round 0.3. This conclusion is confirmed by the observation of the experimental grain displacementload curves presented in Fig. 3. Load (kn) C1 C2 C3 C Grain displacement (mm) Fig. 3 Grain displacement  load curves obtained in the compression tests The Fig. 3 confirm the plastic behaviour recognize to wood under compression parallel to grain and point out a good softening in the grain displacementload curves. Discussion of the Results On the basis of the experimental results, it can be stated the pleasant homogeneity presented by the bending behaviour, especially in terms of elastic modulus. The local modulus of elasticity in bending (E m,l ) presented a CoV equal to 0.11 while the global modulus of elasticity (E m,g ) achieved showed a CoV of In terms of the compression parallel to grain tests results, although the plastic behaviour obtained and the ductile failures achieved, a significant variability was pointed out. Coefficients of variations near of 0.3 were obtained for the elastic modulus and strength. When comparing the experimental results with the values reported in the Portuguese Nationally Determined Parameters of Eurocode 5 (DNA EC5) [3], for the quality class assign in the visual grading performed following NP4305:1995 [2] (Table 3), different conclusions are reached: (1) the bending strength achieved is 21.6% higher than the characteristic value assumed by the National Standard; (2) the mean value obtained for the modulus of elasticity (E m,l ) is 34.2% smaller that the
5 one suggest by DNAEC5; and (3) good agreement between the compression strength value adopted in the DNAEC5 and the experimental results. If the experimental result was MPa, DNAEC5 suggests 24.7 MPa as the characteristics value for the compression strength parallel to the grain. In this standard any value of modulus of elasticity in compression parallel to the grain is presented. Table 3 Mechanical properties of Pinus Pinaster Ait. Class EE [3] Class E m (N/mm 2 ) f m (N/mm 2 ) f c,0 (N/mm 2 ) EE It is important to remember that the values exposed in the DNAEC5 were obtained on specimens free from faults, with nonstructural dimensions and with a moisture content of 12%. It is recognize that the mechanical characterization of wood by means of tests on specimens in small dimension can be inadequate to have reliable and complete information on the structural behaviour of timber elements and structures. For instance, the failure modes obtained in the bending tests conducted are quite different from typical bending failure characteristic of small pieces free from faults, Fig. 4 (a). The existence of knots does not allow the development of the plastic behaviour in the compression side of the cross section (see Fig. 2). Failure append in the tension side and progress rapidly under influence of shear forces without any plastification of the compression side, while the formation of a plastic hinge in the compression side is always obtained in specimens free from faults. In compression, also the existence of faults can determine the failure mode. If in this kind of test the failure mode is more and less constant, is development is always stipulate by the presence of knots, reaction wood, etc., Fig. 4 (b). (a) Bending test B2 (b) Compression test S3 Fig. 4 Failure modes obtained in the experimental work Conclusions With a natural material like wood, so depending of the existence of faults, the mechanical evaluation can not use small specimens free from faults, especially when their presence have the importance showed in this work. Attention has to be moved towards the experimental investigation of the mechanical evaluation of wood elements having structural dimensions and presenting the natural faults recognize to this material. References [1] pren 408:2000: Timber structures Structural timber and glued laminated timber Determination of some physical and mechanical properties, CEN, [2] NP 4305:1995: Structural maritime pine swan timber Visual grading, CT 14 LNEC, [3] NP ENV :1998: Eurocódigo 5  Projecto de estruturas de Madeira. Parte 11: Regras gerais e regras para edifícios. CT 115 LNEC, 1998.
6
Densified Veneer Wood for Notched Joints in Timber Concrete Composite Structures
Densified Veneer Wood for Notched Joints in Timber Concrete Composite Structures 1 Summary Dias, A.M.P.G. (alfgdias@dec.uc.pt) Assistant Professor University of Coimbra CoimbraPortugal Kuilen, J.W.G.,
More informationDEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS
1 th Canadian Masonry Symposium Vancouver, British Columbia, June 5, 013 DEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS Vladimir G. Haach 1, Graça Vasconcelos and Paulo
More informationLOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO THE GRAIN
LOADCARRYING CAPACITY OF AXIALLY LOADED RODS GLUEDIN PERPENDICULAR TO TE GRAIN Prof. Dr.Ing..J. Blaß, Dipl.Ing. B. Laskewitz Universität Karlsruhe (T), Germany Abstract Gluedin rods have been used
More informationUnit 48: Structural Behaviour and Detailing for Construction. Chapter 13. Reinforced Concrete Beams
Chapter 13 Reinforced Concrete Beams Concrete is a material strong in its resistance to compression, but very weak indeed in tension. good concrete will safely take a stress upwards of 7 N/mm 2 in compression,
More informationBuilding Project using PostTensioning
Building Project using PostTensioning Paulo Marques 1 Resume Nowadays building flexibility is an aspect to be taken into account at the idealization and project stages. The number of buildings that throughout
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationOptimising plate girder design
Optimising plate girder design NSCC29 R. Abspoel 1 1 Division of structural engineering, Delft University of Technology, Delft, The Netherlands ABSTRACT: In the design of steel plate girders a high degree
More informationNUMERICAL ANALYSIS OF GLULAM BEAMS WITHOUT AND WITH GFRP REINFORCEMENT
10th International Conference on Composite Science and Technology ICCST/10 A.L. Araújo, J.R. Correia, C.M. Mota Soares, et al. (Editors) IDMEC 2015 NUMERICAL ANALYSIS OF GLULAM BEAMS WITHOUT AND WITH GFRP
More informationTensile Testing. Objectives
Laboratory 1 Tensile Testing Objectives Students are required to understand the principle of a uniaxial tensile testing and gain their practices on operating the tensile testing machine. Students are able
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationENGINEERING SCIENCE H1 OUTCOME 1  TUTORIAL 3 BENDING MOMENTS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P
ENGINEERING SCIENCE H1 OUTCOME 1  TUTORIAL 3 BENDING MOMENTS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL 4 H1 FORMERLY UNIT 21718P This material is duplicated in the Mechanical Principles module H2 and those
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationCost Action FP1101 Assessment, Reinforcement and Monitoring of Timber Structures
Cost Action FP1101 Assessment, Reinforcement and Monitoring of Timber Structures Short Term Scientific Mission Report: ASSESSMENT AND DIAGNOSIS OF AN ANCIENT COLLAR TRUSS BY MEANS OF VISUAL GRADING AND
More informationSPECIFICATIONS, LOADS, AND METHODS OF DESIGN
CHAPTER Structural Steel Design LRFD Method Third Edition SPECIFICATIONS, LOADS, AND METHODS OF DESIGN A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part II Structural
More informationHardened Concrete. Lecture No. 14
Hardened Concrete Lecture No. 14 Strength of Concrete Strength of concrete is commonly considered its most valuable property, although in many practical cases, other characteristics, such as durability
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationσ = F / A o Chapter Outline Introduction Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? and Tension Compression Shear Torsion Elastic deformation Chapter Outline Introduction To understand and describe how materials
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS
MECHANICS OF SOLIDS  BEAMS TUTORIAL 2 SHEAR FORCE AND BENDING MOMENTS IN BEAMS This is the second tutorial on bending of beams. You should judge your progress by completing the self assessment exercises.
More informationLocal buckling of plates made of high strength steel
Local buckling of plates made of high strength steel Tapani Halmea, Lauri Huusko b,a, Gary Marquis a, Timo Björk a a Lappeenranta University of Technology, Faculty of Technology Engineering, Lappeenranta,
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationReinforced Concrete Design SHEAR IN BEAMS
CHAPTER Reinforced Concrete Design Fifth Edition SHEAR IN BEAMS A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part I Concrete Design and Analysis 4a FALL 2002 By Dr.
More informationThe University of Birmingham (Live System)
The University of Birmingham (Live System) Behaviour of Structural Insulated Panels (SIPs) under both shortterm and longterm loadings Yang, Jian; Rungthonkit, Prathan Document Version Author final version
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationShear Reinforcements in the Reinforced Concrete Beams
American Journal of Engineering Research (AJER) eissn : 23200847 pissn : 23200936 Volume02, Issue10, pp191199 www.ajer.org Research Paper Open Access Shear Reinforcements in the Reinforced Concrete
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationStatics and Mechanics of Materials
Statics and Mechanics of Materials Chapter 41 Internal force, normal and shearing Stress Outlines Internal Forces  cutting plane Result of mutual attraction (or repulsion) between molecules on both
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationDESIGN OF SLABS. 3) Based on support or boundary condition: Simply supported, Cantilever slab,
DESIGN OF SLABS Dr. G. P. Chandradhara Professor of Civil Engineering S. J. College of Engineering Mysore 1. GENERAL A slab is a flat two dimensional planar structural element having thickness small compared
More informationFatigue :Failure under fluctuating / cyclic stress
Fatigue :Failure under fluctuating / cyclic stress Under fluctuating / cyclic stresses, failure can occur at loads considerably lower than tensile or yield strengths of material under a static load: Fatigue
More informationChapter 5: Tool Dynamometers
Chapter 5: Tool Dynamometers LEARNING OBJECTIVES Different types of transducers used in Dynamometers Design Requirements Types of Dynamometers 
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More informationEFFECTIVE BENDING CAPACITY OF DOWELTYPE FASTENERS
EFFECTIVE BENDING CAPACITY OF DOWELTYPE FASTENERS Hans Joachim Blass 1), Adriane Bienhaus 1) and Volker Krämer 1) 1) Lehrstuhl für Ingenieurholzbau und Baukonstruktionen, University of Karlsruhe, Germany
More informationStructural fire design Eurocode 51.2 Timber structures
Background and Applications Brussels, 1820 February 2008 Dissemination of information workshop 1 Structural fire design Eurocode 51.2 Timber structures Jochen Fornather Austrian Standards Institute jochen.fornather@onnorm.at
More informationTHE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE
THE DETERMINATION OF DELAMINATION STRAIN ENERGY RELEASE RATE OF COMPOSITE BIMATERIAL INTERFACE Jaroslav Juracka, Vladimir Matejak Brno University of Technology, Institute of Aerospace Engineering juracka@fme.vutbr.cz;
More informationOverview of Topics. StressStrain Behavior in Concrete. Elastic Behavior. NonLinear Inelastic Behavior. Stress Distribution.
StressStrain Behavior in Concrete Overview of Topics EARLY AGE CONCRETE Plastic shrinkage shrinkage strain associated with early moisture loss Thermal shrinkage shrinkage strain associated with cooling
More informationFLEXURAL PERFORMANCE OF RC BEAMS STRENGTHENED WITH PRESTRESSED CFRP SHEETS
FLEXURAL PERFORMANCE OF RC BEAMS STRENGTHENED WITH PRESTRESSED CFRP SHEETS Piyong Yu, Pedro F. Silva, Antonio Nanni Center for Infrastructure and Engineering Studies Department of Civil, Architectural,
More informationStresses in Beam (Basic Topics)
Chapter 5 Stresses in Beam (Basic Topics) 5.1 Introduction Beam : loads acting transversely to the longitudinal axis the loads create shear forces and bending moments, stresses and strains due to V and
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationOptimum proportions for the design of suspension bridge
Journal of Civil Engineering (IEB), 34 (1) (26) 114 Optimum proportions for the design of suspension bridge Tanvir Manzur and Alamgir Habib Department of Civil Engineering Bangladesh University of Engineering
More informationANALYSIS FOR BEHAVIOR AND ULTIMATE STRENGTH OF CONCRETE CORBELS WITH HYBRID REINFORCEMENT
International Journal of Civil Engineering and Technology (IJCIET) Volume 6, Issue 10, Oct 2015, pp. 2535 Article ID: IJCIET_06_10_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=6&itype=10
More informationLOAD DEFLECTION DIAGRAM OF OVERREINFORCED CONCRETE BEAMS
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDIFICATIO Publishers, D79104 Freiburg, Germany LOAD DEFLECTION DIAGRAM OF OVERREINFORCED CONCRETE BEAMS A. Bascoul Laboratoire Materiaux
More informationReinforced Concrete Design to BS8110 Structural Design 1 Lesson 5
Lesson 5: Deflection in reinforced concrete beams Content 4.1 Introduction 4. Definitions 4..1 Tension 4.. Compression 4.3 Initial sizing 4.3.1 Worked example 4.4 Reinforcement details 4.5 Anchorage at
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationLab for Deflection and Moment of Inertia
Deflection and Moment of Inertia Subject Area(s) Associated Unit Lesson Title Physics Wind Effects on Model Building Lab for Deflection and Moment of Inertia Grade Level (1112) Part # 2 of 3 Lesson #
More informationBehavior of high strength structural steel at elevated temperatures
University of Wollongong Research Online Faculty of Engineering  Papers (Archive) Faculty of Engineering and Information Sciences 2006 Behavior of high strength structural steel at elevated temperatures
More informationPerformance Evaluation of Bamboo Reinforced Concrete Beam
Compressive (MPa) Setting Time Fineness International Journal of Engineering & Technology IJETIJENS Vol: 11 No: 04 113 Performance Evaluation of Bamboo Reinforced Concrete Beam M. M. Rahman, M. H. Rashid,
More informationGLUED TIMBERCONCRETE BEAMS ANALYTICAL AND NUMERICAL MODELS FOR ASSESSMENT OF COMPOSITE ACTION
Engineering Review Vol. Issue 9. GLUED TIMBERCONCRETE BEAMS ANALYTICAL AND NUMERICAL MODELS FOR ASSESSMENT OF COMPOSITE ACTION L. Škec A. Bjelanović * G. Jelenić Faculty of Civil Engineering University
More informationPage 1 of 18 28.4.2008 Sven Alexander Last revised 1.3.2010. SBProduksjon STATICAL CALCULATIONS FOR BCC 250
Page 1 of 18 CONTENT PART 1 BASIC ASSUMPTIONS PAGE 1.1 General 1. Standards 1.3 Loads 1. Qualities PART ANCHORAGE OF THE UNITS.1 Beam unit equilibrium 3. Beam unit anchorage in front..1 Check of capacity..
More informationSeismic analysis of a 2storey log house Jorge M. Branco a, Paulo B. Lourenço b, Chrysl A. Aranha c
Seismic analysis of a 2storey log house Jorge M. Branco a, Paulo B. Lourenço b, Chrysl A. Aranha c ISISE, Department of Civil Engineering, University of Minho, Guimarães, Portugal a jbranco@civil.uminho.pt,
More informationNanping Weishi LVL Scaffold Plank Brochure
Nanping Weishi LVL Scaffold Plank Brochure Weishi Wood Inudstry Co., Ltd. is PFS Certified Mill. Weishi Planks are OSHA Compliant Products. Weishi Team is Aimed to Offer You the Best Quality and Service.
More informationFOURPLATE HEB100 BEAM SPLICE BOLTED CONNECTIONS: TESTS AND COMMENTS
FOURPLATE HEB BEAM SPLICE BOLTED CONNECTIONS: TESTS AND COMMENTS M.D. Zygomalas and C.C. Baniotopoulos Institute of Steel Structures, Aristotle University of Thessaloniki, Greece ABSTRACT The present
More informationBending Stress in Beams
93673600 Bending Stress in Beams Derive a relationship for bending stress in a beam: Basic Assumptions:. Deflections are very small with respect to the depth of the beam. Plane sections before bending
More informationINTRODUCTION TO BEAMS
CHAPTER Structural Steel Design LRFD Method INTRODUCTION TO BEAMS Third Edition A. J. Clark School of Engineering Department of Civil and Environmental Engineering Part II Structural Steel Design and Analysis
More informationAnalysis of Reinforced Concrete Beams Strengthened with Composites. Subjected to Fatigue Loading
Analysis of Reinforced Concrete Beams Strengthened with Composites Subjected to Fatigue Loading By Christos G. Papakonstantinou, Perumalsamy. Balaguru and Michael F. Petrou Synopsis: Use of high strength
More informationFullScale Load Testing of Steel Strutting System. For. Yongnam Holding Limited
Report on FullScale Load Testing of Steel Strutting System For Yongnam Holding Limited Prepared by Dr Richard Liew PhD, MIStrutE, CEng, PE(S pore) Department of Civil Engineering National University of
More informationSolution for Homework #1
Solution for Homework #1 Chapter 2: Multiple Choice Questions (2.5, 2.6, 2.8, 2.11) 2.5 Which of the following bond types are classified as primary bonds (more than one)? (a) covalent bonding, (b) hydrogen
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationproduct manual H3030A, H3032A, H3033A Concrete Beam Tester
product manual 11.09 H3030A, H3032A, H3033A Concrete Beam Tester Introduction These selfcontained portable concrete beam testers accurately and easily determine flexural strengths of 6 x 6" crosssection
More informationModule 3. Limit State of Collapse  Flexure (Theories and Examples) Version 2 CE IIT, Kharagpur
Module 3 Limit State of Collapse  Flexure (Theories and Examples) Lesson 4 Computation of Parameters of Governing Equations Instructional Objectives: At the end of this lesson, the student should be able
More informationThe University of Bradford Institutional Repository
The University of Bradford Institutional Repository http://bradscholars.brad.ac.uk This work is made available online in accordance with publisher policies. Please refer to the repository record for this
More informationCOMPARISON OF STRESS BETWEEN WINKLERBACH THEORY AND ANSYS FINITE ELEMENT METHOD FOR CRANE HOOK WITH A TRAPEZOIDAL CROSSSECTION
COMPARISON OF STRESS BETWEEN WINKLERBACH THEORY AND ANSYS FINITE ELEMENT METHOD FOR CRANE HOOK WITH A TRAPEZOIDAL CROSSSECTION Yogesh Tripathi 1, U.K Joshi 2 1 Postgraduate Student, 2 Associate Professor,
More informationTechnical Notes 3B  Brick Masonry Section Properties May 1993
Technical Notes 3B  Brick Masonry Section Properties May 1993 Abstract: This Technical Notes is a design aid for the Building Code Requirements for Masonry Structures (ACI 530/ASCE 5/TMS 40292) and Specifications
More informationAdam Zaborski handouts for Afghans
Tensile test Adam Zaborski handouts for Afghans Outline Tensile test purpose Universal testing machines and test specimens Stressstrain diagram Mild steel : proportional stage, elastic limit, yielding
More informationPhysics 172H. Lecture 6 BallSpring Model of Solids, Friction. Read
Physics 172H Lecture 6 BallSpring Model of Solids, Friction Read 4.14.8 Model of solid: chemical bonds d radial force (N) 0 F linear If atoms don t move too far away from equilibrium, force looks like
More informationDynamic Measurement of Brake Pads Material Parameter
VDA Dynamic Measurement of Brake Pads Material Parameter 315 This nonbinding recommendation by the German Association of the Automotive Industry (VDA) has the following objectives: This standard treats
More informationCarbon Fiber Reinforced Polymer (CFRP) as Reinforcement for Concrete Beam
Carbon Fiber Reinforced Polymer (CFRP) as Reinforcement for Concrete Beam Norazman Mohamad Nor 1, Mohd Hanif Ahmad Boestamam, Mohammed Alias Yusof 3 1,3 Universiti Pertahanan Nasional Malaysia, 57000 Kuala
More informationVersion default Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 Responsable : François HAMON Clé : V6.03.161 Révision : 9783
Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 SSNP161 Biaxial tests of Summarized Kupfer: Kupfer [1] was interested to characterize the performances of the concrete under biaxial
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More informationSheet metal operations  Bending and related processes
Sheet metal operations  Bending and related processes R. Chandramouli Associate DeanResearch SASTRA University, Thanjavur613 401 Table of Contents 1.QuizKey... Error! Bookmark not defined. 1.Bending
More informationTECHNICAL CHARACTERISTICS
TECHNICAL CHARACTERISTICS The technical characteristics of KLH crosslaminated timber panels are: Board Format Max. length 16.50m For UK transportation, we would recommend a maximum length of 13.50m Board
More informationTesting Anchors in Cracked Concrete
Testing Anchors in Cracked Concrete Guidance for testing laboratories: how to generate cracks BY ROLF ELIGEHAUSEN, LEE MATTIS, RICHARD WOLLMERSHAUSER, AND MATTHEW S. HOEHLER ACI Committee 355, Anchorage
More informationAssistant Professor of Civil Engineering, University of Texas at Arlington
FRC Performance Comparison: Direct Tensile Test, Beam Type Bending Test, and Round Panel Test Shih Ho Chao (Presenting Author) Assistant Professor of Civil Engineering, University of Texas at Arlington
More informationFlexural Strength of Concrete (The Modulus of Rupture Test)
Revised 09063, WKS Datasheet No. 7.6a & 7.6b MOHAWK COLLEGE OF APPLIED ARTS AND TECHNOLOGY BUILDING AND CONSTRUCTION SCIENCES DEPARTMENT Flexural Strength of Concrete (The Modulus of Rupture Test) INTRODUCTION
More informationExperimental Investigation on Shear Cracking Behavior in Reinforced Concrete Beams with Shear Reinforcement
Journal of Advanced Concrete Technology Vol. 7, No. 1, 7996, February 29 / Copyright 29 Japan Concrete Institute 79 Scientific paper Experimental Investigation on Shear Cracking Behavior in Reinforced
More informationFibre Reinforced Concrete Beams Subjected to Air Blast Loading
 1  ibre Reinforced Concrete Beams Subjected to Air Blast Loading Johan Magnusson Ph.D. student Division of Concrete Structures Royal Institute of Technology SE1 44 Stockholm, Sweden Email: Johan.Magnusson@byv.kth.se
More informationThe Material Properties of Cement Paste with Fly Ash Exposed to High Temperatures
The Material Properties of Cement Paste with Fly Ash Exposed to High s PAVEL PADEVĚT, ROMANA LOVICHOVÁ Department of Mechanics Czech Technical University in Prague Thákurova 7, 166 29, Prague 6 CZECH REPUBLIC
More informationDesign MEMO 54a Reinforcement design for RVK 41
Page of 5 CONTENTS PART BASIC ASSUMTIONS... 2 GENERAL... 2 STANDARDS... 2 QUALITIES... 3 DIMENSIONS... 3 LOADS... 3 PART 2 REINFORCEMENT... 4 EQUILIBRIUM... 4 Page 2 of 5 PART BASIC ASSUMTIONS GENERAL
More informationModule 2. Analysis of Statically Indeterminate Structures by the Matrix Force Method. Version 2 CE IIT, Kharagpur
Module Analysis of Statically Indeterminate Structures by the Matrix Force Method esson 11 The Force Method of Analysis: Frames Instructional Objectives After reading this chapter the student will be able
More informationTSL Professional Services
Report For: Laboratory #: 40287605 5375 Edgeway Drive, ALLENDALE, MI, USA Report Date: December 21, 2005 49401 Received Date: November 3, 2005 Phone: 616 875 7725 Fax: 616 875 6009 Customer P.O. #: COD
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL TUTORIAL 4  COMPLEMENTARY SHEAR STRESS
MECHANICS OF SOLIDS  BEAMS TUTORIAL TUTORIAL 4  COMPLEMENTARY SHEAR STRESS This the fourth and final tutorial on bending of beams. You should judge our progress b completing the self assessment exercises.
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationMECHANICAL PROPERTIES OF STRUCTURAL STEEL AT ELEVATED TEMPERATURES AND AFTER COOLING DOWN
MECHANICAL PROPERTIES OF STRUCTURAL STEEL AT ELEVATED TEMPERATURES AND AFTER COOLING DOWN Jyri OUTINEN and Pentti MÄKELÄINEN Laboratory of Steel Structures, Department of Civil and Environmental Engineering,
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More information16. BeamandSlab Design
ENDP311 Structural Concrete Design 16. BeamandSlab Design BeamandSlab System How does the slab work? L beams and T beams Holding beam and slab together University of Western Australia School of Civil
More informationEDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME 2 ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS
ENGINEERING COMPONENTS EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES OUTCOME ENGINEERING COMPONENTS TUTORIAL 1 STRUCTURAL MEMBERS Structural members: struts and ties; direct stress and strain,
More informationInsitu Load Testing to Evaluate New Repair Techniques
Insitu Load Testing to Evaluate New Repair Techniques W.J. Gold 1 and A. Nanni 2 1 Assistant Research Engineer, Univ. of Missouri Rolla, Dept. of Civil Engineering 2 V&M Jones Professor, Univ. of Missouri
More informationFigure 1. Oneway slab design (dimensions are in mm) Figure 2. Twoway slab design (dimensions are in mm)
BEHAVIOUR OF INNOVATIVE FIBRE COMPOSITE SANDWICH PANELS UNDER POINT LOADING M.M. Islam 1, T. Aravinthan 1 and G. Van Erp 2 1 Centre of Excellence in Engineered Fibre Composites, Faculty of Engineering
More informationThe following sketches show the plans of the two cases of oneway slabs. The spanning direction in each case is shown by the double headed arrow.
9.2 Oneway Slabs This section covers the following topics. Introduction Analysis and Design 9.2.1 Introduction Slabs are an important structural component where prestressing is applied. With increase
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationMODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS
MODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS Bjørn Konradsen 1 Technological Analyses Centre, Hybrid Underwater Cables, Nexans Norway Steinar V. Ouren Material
More information7.2.4 Seismic velocity, attenuation and rock properties
7.2.4 Seismic velocity, attenuation and rock properties Rock properties that affect seismic velocity Porosity Lithification Pressure Fluid saturation Velocity in unconsolidated near surface soils (the
More informationbi directional loading). Prototype ten story
NEESR SG: Behavior, Analysis and Design of Complex Wall Systems The laboratory testing presented here was conducted as part of a larger effort that employed laboratory testing and numerical simulation
More information